Dear Label_Name,

Greetings! I hope you are well.

I am writing on behalf of an international publishing house, Science and Education Publishing, USA (http://www.sciepub.com).

Science and Education Publishing (SciEP) is a multidisciplinary open access publisher of Journals covering the fields of Science, Technology and Medicine. All SciEP publications are subject to high-quality peer review, editorial and production processes and are freely available online.

Welcome to the April, 2013 edition of SciEP newsletter, providing monthly summaries of articles on science & education related topics of interest to scientist and professionals. The mission of our journals is to provide an open access forum for publishing new findings on issues pertinent to scientific and academic field. We also invite you to submit original research papers, review articles, short reports, or case studies are considered for publication in our Multidisciplinary Journals.

American Journal of Public Health Research
DOI: 10.12691/ajphr-1-1-3

The Implementation of a Tele-Homecare System with Service Oriented Architecture and HL7 Message Transmission Standard
Ching-Sung Wang

American Journal of Medical and Biological Research
DOI: 10.12691/ajmbr-1-1-2

The Influence of Ethanol on Pyruvate Kinases Activity in Vivo, in Vitro, in Silico
Lelevich Sergey Vladimirovich, Khrustalev Vladislav Victorovich, Barkovsky Eugene Victorovich, Shedogubova Tatyana Aleksandrovna

American Journal of Medical Sciences and Medicine
DOI: 10.12691/ajmsm-1-1-1

Clinical and Histological Features in Wegener Granulomatosis
Li Cavoli Gioacchino, Passantino Rita, Bono Luisa, Tortorici Calogera, Ferrantelli Angelo, Giammarresi Carlo, Rotolo Ugo

American Journal of Infectious Diseases and Microbiology
DOI: 10.12691/ajidm-1-1-2

The Curse of Lymphatic Filariasis: Would the Continual Use of Diethylcarbamazine Eliminate this Scourge in Papua New Guinea?
Anne Lanham, Lillian Mwanri

We have released issues of some journals on February 2013.
American Journal of Public Health Research
American Journal of Medical Sciences and Medicine
American Journal of Medical and Biological Research
American Journal of Pharmacological Sciences
American Journal of Clinical Medicine Research
American Journal of Nursing Research
American Journal of Cancer Prevention
American Journal of Medicine Studies
American Journal of Infectious Diseases and Microbiology
American Journal of Cardiovascular Disease Research
American Journal of Biomedical Research
American Journal of Mechanical Engineering
American Journal of Microbiological Research
Journal of Preventive Medicine
American Journal of Food and Nutrition
American Journal of Hypertension Research
American Journal of Sports Science and Medicine
Journal of Cancer Research and Treatment
American Journal of Zoological Research
Journal of Biomedical Engineering and Technology
American Journal of Microbiological Research
Biomedical Science and Engineering

We are pleased to announce that submissions are now being accepted for peer review for all the journals across all our subject areas in SciEP.

Please submit your manuscript via our online submission system:
http://www.sciepub.com/author/signin

To unsubscribe from our mailing list, please click on the following link: unsubscribe

I am looking forward to hearing from you.

Kind regards,

David Rain
Email:join@sciepub.com
Science and Education Publishing (http://www.sciepub.com)

Turnability of the Plasmonic Response of the Gold Nanoparticles in Infrared Region

A Sambou, B D Ngom*, L Gomis, A C Beye

Laboratoire de Photonique et de Nano-Fabrication, Faculté des sciences et Techniques Université Cheikh Anta Diop de Dakar (UCAD) B.P. 25114 Dakar-Fann Dakar, Senegal

Abstract: We report on the modulation of the optical properties namely the Surface Plasmon Resonance (SPR) of gold nanoparticles core-shell as function of the surrounding medium (water, ethanol). We have study two different combinations (1) silica thin film coating gold nanospheres and (2) gold thin film coating silica nanoparticles. The optical model used is based on Mie theory by considering spherical gold nanoparticles core-shell and the simulation is done using Matlab program. The results show an important influence of the surrounding medium and the size of the core as well as the shell thickness, on the optical properties with a redshift of the Surface Plasmon Resonance (SPR). By using Mie theory and Drude model for the simulation of the Surface Plasmon Resonance model of spherical nanoparticles showed that for the control of the Surface Plasmon Resonance of the gold thin film coating silica nanoparticles it is important to considered three parameters (i) the size of core (ii) the surrounding medium and (iii) shell thickness, which enable the turning of the SPR through the near infrared; where as gold nanosphere coated by silica results has a maximum wavelength at 530 nm, this Plasmon peak corresponding a R₁/d ratio of 1.6. Thus, this work enabled optimizing core-shell structure with well-controlled sizes for biomedical application.

Keywords: Nanospheres particles, Nanospheres, shell thickness, Surface Plasmon Resonance

Citation: A Sambou, B D Ngom, L Gomis, A C Beye, Turnability of the Plasmonic Response of the Gold Nanoparticles in Infrared Region. American Journal of Nanomaterials, 4 (3). 63-69. January 2016. doi:10.12691/ajn-4-3-3

1. Introduction

Spite the significant efforts made in medical research for cancer treatments, it remains one of the major causes of death in the world. Various methods of treatment bringing into play a laser, microwaves, radio frequencies…etc, were tested for local heat treatment of cancerous area to destroy it. The cancer cells are naturally more sensitive to the radiation than the normal cells. However, these treatments by microscopic, cause not only the destruction of the tumoral cell but also the destruction of healthy surrounding cells and thus produce many side effects [1].

Nanosciences and Nanotechnologies open new ways towards better, adapted and more targeted treatment. Indeed, du to their sizes effects, nanoparticles can be utilized for the simultaneous removal of cancer. The nanotechnology allows the production of nanoparticles, which is at the origin of Surface Plasmon Resonance [2].

Surface Plasmon Resonance is collective excitations of the electrons at the interface between a conductor and an insulator and it is described by evanescent electromagnetic waves that are not necessarily located at the interface [3,4].

Noble metal nanoparticles are of advantages because they are not degraded under laser irradiation and allow also an important reduction laser power, this is du to their high absorption cross section [5]. Noble metals nanoparticles present remarkable optical properties, which explain all the interest of their usage. Besides their optical properties, noble metal nanoparticles have found applications in many different fields; we can quote electronics, optics, catalysis and nanomedicine [3,6]. Gold nanoparticles have numerous promising applications in nanomedicine field, they are used to produce thermal tumor ablation and new therapeutic agents.

Most of these applications use the unique optical properties of gold nanoparticles, which is the Surface Plasmon Resonance [4], photoluminescence and Surface Enhanced Raman Scattering (SERS) effect [2]. Gold plasmonic i.e. SPR nanoparticles are widely used in biological applications, such as contrast agents for cancer detection, photothermal therapy [7]. Properties of SPR are used to the diagnostic of cancer, for example gold nanoshells with solid silica cores have great potential for cancer photothermal therapy [8].

With regard to the application of the nanoparticles in biology, gold nanoparticles are the metal nanoparticles most frequently used due of their properties. First of all, gold is not toxic. Like silver and copper, gold presented a strong absorption in visible spectrum, called the Plasmon band. Gold nanoparticles resonance is localized in visible spectrum [9], Christina Graf and co-workers, affirmed that the Surface Plasmon Resonance (SPR) of gold nanospheres of 5 nm of radius embed in water are localized at 520 nm [10] whereas SPR of silver nanospheres is localized towards 410 nm [11,12]. Broader Nikolai G. khlebtsov reported gold nanospheres in water having radius in the interval 5 nm < R < 20 nm, their Plasmon resonance is observed at 520 nm [13]. The most important feature of the SPR is its position in the spectrum and its band intensity. To enable biomedical applications, the resonance plasmon frequency of the nanoparticles should be however in the near infrared (NIR) region [14]. Principal approach to enable use of nanoparticles for biomedical application is to fabric nanostructures (core/shell). Core/shell nanoparticles are a new type of nanoparticle composed of a dielectric core such as metallic oxide or polymer coated with metallic layer, which is typically gold. P. Mulvaney and al [15] established absorption of a film of nanoparticles core shell Au/SiO₂ at 525 nm. By rationally tuning the cores as well as the shells of such materials, a range of core-shell nanoparticles can be produced with tailorable properties that can play important roles in various applications in medicine for cancer diagnostic and offer sustainable solutions to current diagnostic cancer problems. Indeed, the SPR wavelength depends on the nanoparticles shape (sphere, rods, cubic…), size and local environment [2,4,6].

In this work, we have simulated the absorption cross-section of spherical core/shell nanoparticle using Matlab like simulation program. Nanospherical gold is characterized by appearance of only one Plasmon band [2,16]. Two models were used to explain the physical aspect of Surface Plasmon Resonance: Drude-Maxwell model [2,17] and Mie theory [2,18]. We used the solution of Maxwell’s equations for spherical particles using Mie-Drude theory. According to this theory, we can calculate the optical cross section area, using MATLAB 2011 software for different materials such as gold nanospheres and core-shell nanostructures.

2. Material and Methods

According to M. M. Alvarez et al. [19], when the noble metal particles (gold, silver and copper) are subjected to an electric field, the dielectric function decomposed in two terms: an inter-band contribution (IB), corresponding to the response of 5d electron and an intra-band contribution (ID) or contribution of free electrons. These transitions are in the infrared range. According to the generalized Drude theory, the permittivity of the particle can be written as follows:

[picture] | (1)

And the real (εr) and imagery (εi) part of the dielectric function are respectively given by equations (2) and (3) [20,21].

[picture] | (2)

[picture] | (3)

Inter-bands contributions are taken from the literature (see Table 1) and intra-bands values are defined by the equations (4) and (5).

[picture] | (4)

[picture] | (5)

Table 1. Optical parameters of gold

For metals at near-infrared frequencies, these equations become (6) and (7).

[picture] | (6)

[picture] | (7)

Where ε∞, the high frequency is limit dielectric constant given in the literature, λp is the plasma wavelength given in the literature and τr is relaxation time given by equation (8).

[picture] | (8)

Where is the electron lifetime in seconds and C is the velocity of light (C =8*10⁸ m/s).

For metallic oxide and/or polymer, the optical parameters n and k which respectively designate the refraction index describing the speed of the wave phase and extinction index describing the absorption of the wave during propagation in the material, are respectively expressed by the following relations (9) and (10).

[picture] | (9)

[picture] | (10)

The real and imaginary parts of the complex dielectric function of the particle εr and εI are related to the dielectric function of core noted εa and the dielectric function of shell noted εb (see Figure 1) by the relations (11) and (12).

[picture] | (11)

[picture] | (12)

Figure 1. Spherical core/shell nanoparticle

The optical parameter (n, k) of SiO₂ data are obtained from E. Palik [22]. In the case of a sphere multi-layer (by example core-shell system) the expression of the absorption cross section is solved on the basis of the Laplace equations. For more detail see article [23] and document [24]. It is assumed that the particle diameter is much smaller than the wavelength of the incident field. Then, we can obtain the absorption cross section from the polarizability defined by equation (13).

[picture] | (13)

From Mie scattering theory the absorption cross section is given by equation (14).

[picture] | (14)

Where ε₀=8.85*10⁻¹² F/m is the permittivity of vacuum and εm is the dielectric constant of surrounding medium (εm=n²) with n is refraction index. The extinction coefficient of a small particle is determined by its absorption σabs=σext; in the general case we have the following relation between the extinction (σext), absorption (σabs) and scattering (σsca) cross section σext =σabs+σsca [13,24].

The constant values taken from the literature and that are necessary for this study, are shown in Table 1 with the corresponding references.

3. Results and Discussion

Nanoparticles can be categorized based on single or multiple materials into simple and core/shell or composite nanoparticles. In general, simple nanoparticles are made from single material whereas core/shell particles are composed of two or more materials. Moreover of gold nanoparticles we have used silica material for the formation of nanoshell particles. According to Maria Vallet Regi and Francisco Balas [29], they report that different silica-bassed materials can be employed for designing devices for biomedicine either for drug delivery systems or for bioactive materials in prosthetic applications. In this study, the spectra extended into from visible to the near infrared region (200-1200 nm) were measured.

3.1. Optical Properties of Single Metal Nanoparticles

Equation (14) can provide the absorption spectra of a metal nanoparticle as function of the particle radius R and the refractive index of the medium in which it is embedded. In Figure 2, we have plotted the absorption spectrum of a particle with a 20 nm radius, embedded in a medium with a refraction index of 1.333 (water).

Figure 2. Absorption cross section of gold nanosphere

Figure 3. Surrounding medium effect on the optical properties

As expected, the spectrum of gold nanosphere reveals one only resonance located around at 515 nm in water, caused by the collective plasma oscillation of the free electron gas. The maximum absorption was obtained at wavelength 515 nm characteristic the formation of gold nanosphere nanoparticles. This value is in good agreement with experiments measure, which has been confirmed our model of studies of the optical response. The simulation results for gold nanopshere resemble the experimental spectrum. According to [30] Azim Akbarzadeh and co-workers are obtained a maximum absorption at 518 nm. Whereas this band can be influences by surrounding medium as shown in Figure 3.

Figure 3 shows the absorption cross-section spectra of gold nanospheres in different medium: water, ethanol and benzyl acid. The refractive indexes used are fixed values: 1.333 (water), 1.359 (ethanol) and 1.538 (benzyl alcohol). The optical properties of the gold nanosphere particles shows that with increasing refraction index the intensity of the Plasmon band increases and absorption shifts toward the higher wavelength region as shown in Figure 3. But also band becomes wider. These three bands are localized at 515 nm, 520 nm and at 540 nm for 1.333, 1.359 and 1.539 for refraction indexes values respectively. These results, allow considering a significant factor, which is the surrounding medium. These results confirmed according to the equation (14) that the dielectric constant of the surrounding medium plays a predominant role in the position of the Plasmon peak and its intensity.

3.2. Optical Properties of Core/Shell Nanostructure

We have coated the gold nanoparticles with silica to study their optical properties. The advantage of these nanostructures (core/shell) is the possibility to modify the resonance Plasmon from visible region to near infrared region, and thus the absorption wavelength by changing the core to shell ratio. For d=0 nm (i.e. without any shell of SiO₂) the Surface Plasmon Resonance of the gold nanoparticles is localized at 515 nm in water and 520 nm in ethanol (bleu curve in Figure 4). We have study two different combinations (1) silica thin film coating on gold nanospheres and (2) gold thin film coating on silica nanoparticles.

3.2.1. Silica Coating on Gold Nanosphere

Figure 4 shows the evolution of the Plasmon band when silica is used as a shell to coat the gold nanoparticle. In this case we have considered a gold core of 30 nm of radius (R₁) and the SiO₂ shell thickness (d) vary from 0 nm to 50 nm. First, the silica shell is known to diminishe the bulk metal conductivity and improves the chemical and physical stability of the core component [31]. Second, silica can be used to block the core surface from making contact with a biological environment and also silica particles produced via the Stöber Method have been shown to be chemically biocompatible [32].

The obtained core/shell nanoparticles are emerged into the two different surrounding mediums (water and ethanol). The non-coated gold nanoparticle (d=0 nm), the gold nanoparticles had a characteristic surface plasmon resonance at a wavelength of 515 nm in water and at 520 nm wavelength in ethanol.

Figure 4 shows globally that all the core/shell nanospheres irrespective to the surrounding medium, their SPRs move toward red shifted but remain in visible region. Therefore the increase into the thickness of the shell increases the Surface Plasmon Resonance wavelength, which is gradually red, shifted and its intensity increases as well.

Figure 4. Absorption cross-section for Au/SiO₂ (core/shell) nanospheres at varying thickness shell at core radius of 30 nm

Table 2. Maximum absorption of the Au/SiO2 (core/shell) nanospheres as function of the core/shell ratio at each surrounding medium (water and ethanol)

As it shown in Figure 4, we remark that the maximum absorption is reach when the silica thichness is between 10 and 20 nm in both mediums and the frequency of resonance is positioned at 530 nm wavelength for the two surrounding medium. After reaching a wavelength of 530 nm, the SPRs are nolonger sensitive to the change into the shell thichness but the plasmon band increased in intensity. After we have looked at the influence of the ratio between the core size and the shell thickness on the SPR wavelength; Table 2 summaries the ratio between size of core and thichness of shell for to reach the maximum absorption. Thus a maximum wavelength of 530 nm is achieved at an R₁/d ratio of 1.6 (Cf. Table 2) irrespective to the surrounding medium. The experimental results reported by Yusuke MORIGUCHI and co-authors [33] have showed a very weak variation of the SPR when it increases silica thickness coated with gold nanosphere. We can also quote the work on references [31] and [34] in which the authors have carried experimental studies on the optical properties of Au/SiO₂ nanoparticles. According to these three references [31,33,34], experimental and simulated data are in reasonable agreement with respect to the SPR position in the visible spectrum.

In summary, the thickness of the silica shell does not modify significantly the plasmon response. When particle is emerged in water, Au/SiO₂ red shifted about of 25 nm and 10 nm in ethanol (see Figure 3). In addition, increase core size give the same results as increasing of shell thickness. After the first step of silica coating on gold, the results show clearly that Au/SiO₂ structure SPRs slightly. Samantha Soulé and al [6] have obtained a redshift (resonance peak toward 800 nm) into their system, by experimental method with the Ag/Au/SiO₂ structure, where in their experiment the core was composed of Ag and Au nanoparticle.

3.2.2. Gold Coating on Silica

In this step, gold is considered as the coating thus the shell and silica nanoparticle the core. The simulation absorption cross section spectra are plotted in Figure 5 and Figure 6, for various shell thichness from 3 nm to 20 nm in different dielectric constants of the surrounding medium. In this party, we report the results obtained for gold nanoshells with (silica core radius/gold shell thichness) parameters of (10-50 nm/4-100 nm). These particles are emerged in surrounding medium of refraction index n=1.333 and n=1.359 which is water and ethanol respectively, all results of simulation are summarized in Table 3.

Figure 5 shows the absorption cross section of SiO₂/Au core/shell nanospheres with six shell thicknesses that are 3 nm, 4 nm, 7 nm, 10 nm, 14 nm and 20 nm. These gold layer are used to coat different size of core, radius of core used in this step are R₁=50 nm, R₁=30 nm, R₁=15 nm and R₁=10 nm.

It is important to notice that silica particles do not show any absorption peak from the visible range to the infrared region. It is interesting to notice a relation between the shell thicknesses, the core size and the SPR wavelength. It is well known that, if the thickness of the shell decreases, resonance wavelength red-shifted and band intensity decrease. Theses results are according to reference [35,36]. But we observe that, on increasing the core size of metallic oxide (i.e. silica), the Surface Plasmon Resonance re-shifted far away and its intensity increases.

For the same shell thickness, core particle with bigger size are highly red-shifted as shown in Figure 6.

Figure 5. Absorption cross section for SiO₂/Au core/shell nanospheres at varying thickness shell in water for different core radius

Figure 6. Absorption cross section for SiO₂ core /Au shell a radius core function

Table 3. Wavelength of the resonance band according with the surrounding environment, shell thickness and size core

The thickness of the shell is fixed at 4 nm and the influence of core particle size is study in water. The core size effect reveals a clear high displacement into the infrared as the radius of core increase.

Surface Plasmon Resonance is located at 990 nm, 820 nm, 670 nm and at 620 nm for the core radius equal to 50 nm, 30 nm, 15 nm and 10 nm, respectively. Therefore the surface plasmon band increase in intensity within the increase of the size of the core. Core size is known to be a very important feature that can significantly influence the physical properties of the material. The result indicates that the Plasmon band of SiO₂/Au is more sensitive to the big nanosphères with a big core.

All simulation results are reported in Table 3 in, which we report on the effect of core size on SPR. The thickness of gold layer shown in Table 3 was estimated to be 4, 7, 10, 14, 20, 30, 40, 50, 60, 70, 80, 90 and 100 nm and study is done in to two surrounding medium as reported into Table 3.

From the results obtained, we can say that silica (core)/gold (shell) SPR can be easily shifted in to near infrared region by simple variation of ratio core radius/shell thickness. As shown in Figure 5 and Table 3, for gold coating silica, according to the nature of the medium and thickness of the gold shell but also size of SiO₂ core material, SiO₂/Au nanosphers absorb light in the near infrared region thus can be use biological applications.

Table 3 shows that more the ratio becomes high, nanosphers particles SPR can be shifted in near infrared region. For example in water, for the ratio SiO₂/Au= 2.5; 3.75; 5; 7.5 and 12.5, these particles have shifted at 620, 670, 730, 820 and at 990 nm, respectively.

In summary, we have studied the general behavior of the Surface Plasmon Resonance on small and large nanoparticles in different surrounding environment. For instance, the location of these resonances of these nanosphers are depending on four parameters which can influences their optical properties (i) the core radius (ii) thickness of shell (iii) surrounding medium (iv) the surface geometry of core-shell configuration.

With the aim to optimize the materials in near infrared region, the results are showed in Table 3. This work shows that the particles with large core give the resonance at longer wavelength more than the small core (Figure 6). When the core size of the particle increases, the Surface Plasmon Resonance becomes red shifted more and more important. Study shows that coating silica as core and gold as shell can be use to turn the gold nanosphers SPR in the near infrared region.

4. Conclusion

In this work we have study the turn-ability of the gold nanoparticle SPR to two different combinations (1) silica thin film coating on gold nanospheres and (2) gold thin film coating on silica nanoparticles. And the SPR have been probed into two different mediums (water and ethanol).

The results show initially that wavelength of plasmon resonance of a simple Au/SiO2 nanosphers does not much depending on the surrounding medium whereas for the SiO₂/Au nanosphers three parameters are considered for the control the optical response of the material: surrounding medium, shell thickness and core size.

Note that the results show that SiO₂/Au nanosphers are composed of a dielectric core of silica covered by a thin gold shell their SPR is highly red-shifted and can be ideal candidates for enhancing cancer treatment, cancer detection. Important remark can be pulled in this study, SiO₂/Au nanosphers with large core absorbed more light.

References

[1]   | S. Eibner, R. A. O. Jaime, B. Lamien, R. Basto, H. R. B. Orlande, O. Fudym, Effet photo-thermique de l’inclusion de nanoparticules dans des matériaux fantômes de milieux biologiques.
[2]   | A. Moores and F. Goettmann, New J. Chem., 30 (2006). 1121-1132.
[3]   | P. Tuersun, Optik 127 (2016). 3466-3470.
[4]   | C. Noguez J. Phys. Chem. C 111 (2007). 3806-3819.
[5]   | P. Chekuri, E. S. Glazer, S. A. Curley, Advanced Drug Delivery Review, 62 (2010). 339-345.
[6]   | S. Soulé, J. Allouche, J-C. Dupin, H. Martinez, Micropoeous and Mesoporous Materials 171 (2013). 72-77.
[7]   | L. R. Hirsch, R. J. Stafford, J. A. Bankson, S. R. Sershen, B. Rivera, R.E. Price, J.D. Hazle, N.J. Halas and J. L. West, Proceedings of the National Academy of Sciences USA, 100 (2003). 13549-13554.
[8]   | C. Wu, C. Yu and M. Chu, International Journal of Nanomedicine 6 (2011). 807-813.
[9]   | M. T. Delapierre, J. Mohamed, S. Mornet, E. Duguet, S. Ravaine, Gold Bulletin (2008). 195-207.
[10]   | C. Graf and A. V Blaaderen, Langmuir 18 (2002). 524-534.
[11]   | V. V. Apyari, S. G. Dmitrienko, Y. A. Zolotov, Sensors and Actuators B 188 (2013). 1109-1115.
[12]   | M. J. Ko, Adv. Mater. Opt. Electron, 8 (1998). 173-180.
[13]   | N. G. Khlebtsov, L. A. Dykman, journal of Quantitative Spectroscopy & Radiative Transfer 111 (2010). 1-35.
[14]   | J. Oh, H. Yoon and J. Park, Biomed Eng Lett 3 (2013). 67-73.
[15]   | P. Mulvaney, L. M. Liz-Marzan, M. Giersig and T. Ung, J. Mater. Chem., 10 (2000). 1259-1270.
[16]   | S. Link and M. El-Sayed, J. Phys. Chem. B 103 (1999). 4212-4217.
[17]   | A. S. Iglesias, I. P. Santos, J. P. Juste, B. R. Gonzalez, F.J. G. de Abajo and L. M.L. Marzan, ADVANCED MATERIALS 18 (2006). 2529-2534.
[18]   | H. Horvath, Journal of Quantitative Spectroscopy & Radiative Transfer 110 (2009). 787-799.
[19]   | M. M. Alvarez, J. T. Khoury, T. G. Schaaff, M. N. Shafigullin, I. Vezmar and R. L Whetten, B 101 (1997). 3706-3712.
[20]   | P. B. Johnson and R. W. Christy, PHYSICAL REVIEW B 6 (1972). 4370-4379.
[21]   | M. A. Ordal, L. L. Long, R. J. Bell, S. E. Bell, R. R. Bell, R. W. Alexander, Jr., And C. A. Ward, Applied optics 22 (1983). 1099-1120.
[22]   | E. Palik, Handbook of Optical Constants of Solids Vol I, Academic Press, Orlando, pp. 759.
[23]   | G. Weng, J. Li, J. Zhu and J. Zhao, Colloids and Surfaces A: Physicochem. Eng. Aspects 369 (2010). 253-259.
[24]   | T. A. Erickson and J. W. Tunnell, Gold Nanoshell in Biomedical Applications.
[25]   | B. R. Cooper, H. Ehrenreich and H. R. Philipp, Phys. Re 138 (1965). 494-507.
[26]   | S. Berthier and J. Lafait, J. Physique 47 (1986). 249-257.
[27]   | P. G. Etchegoin, E. C. Le Ru and M. Meyer, J. Chem. Phys. 125 (2006). 164705.
[28]   | D. Rioux, S. Vallières, S. Besner, P. Munoz, E. Mazur and M. Meunier, Adv. Optical Mater (2013). 1-7.
[29]   | M. Vallet-Regi and F. Balas, Open Biomedical Engineering Journal 2 (2008). 1-9.
[30]   | A. Akbarzadeh, D. Zare, A. Farhangi, M. R. Mehrabi, D. Norouzian, American Journal of Applied Sciences 6 (2009). 691-695.
[31]   | R. G. Chaudhuri and S. Paria, CHEMICAL REVIEWS 112 (2012). 2373-2433.
[32]   | H. Zhang, DR Dunphy, X. Jiang, H. Meng, B. Sun, D. Tarn, M. Xue, X. Wang, S. Ling, Z. Ji, R. Li, FL. Garcia, J. Yang, ML. kirk, T. Xia, JL. Zink, A. Nel, CJ. Brinker, J AM Chem Soc. 134 (2012). 15790-15804.
[33]   | Y. MORIGUCHI, X. MENG, K. FUJITA, S. MURAI and K. TANAKA, J. Jpn. Soc. Powder Metallurgy 60 (2012). 49-54.
[34]   | B. Sadtler and A. Wei, CHEM. COMMUN (2002). 1604-1605.
[35]   | S. J. Oldenburg, R. D. Averitt, S. L. Westcott, N. J. Halas, Chem. Phys. Lett 288 (1998). 243.
[36]   | C. Loo, A. Lin, L. Hirsch, M-H. Lee, J. Barton, N. Halas, J. West and R. Drezek, Technology in Cancer Research & Treatment 3 (2004). 33-40.